Mechanical, Durability and Microstructure Properties of ... paper... Mechanical, Durability and...
Embed Size (px)
Transcript of Mechanical, Durability and Microstructure Properties of ... paper... Mechanical, Durability and...
Mechanical, Durability and Microstructure Properties of Cold Asphalt Emulsion Mixtures with Different Types of Filler
Ahmed I. Nassar1*, Mahmoud Khashaa Mohammed2, Nicholas Thom1 and Tony Parry1
1Nottingham Transportation Engineering Centre, Department of Civil Engineering, Faculty of
Engineering, University of Nottingham, University Park, Nottingham NG7 2RD, UK.
2Civil Engineering Department, Faculty of Engineering, University of Anbar, Anbar
*Corresponding author: E-mail: firstname.lastname@example.org, email@example.com.
The primary aim of this study is to investigate the enhancement of Cold Asphalt Emulsion
Mixtures (CAEMs) using binary and ternary blended fillers (BBF and TBF), including an in-
depth assessment of the microstructure. Ordinary Portland cement (OPC), fly ash (FA) and
ground granulated blast furnace slag (GGBS) were used for the BBF while silica fume (SF) was
added to the BBF to obtain TBF. The mechanical and durability results indicated that the TBF
was more suitable than the BBF for the production of CAEMs. The microstructural assessment
indicated that the effect of BBF on the internal microstructure of CAEMs was slightly negative
and more noticeable in CAEMs containing FA. It is proposed that the addition of SF to BBF
mixtures can eliminate the delay in formation of hydration products caused by the bitumen
emulsion. Overall, the research suggests that the use of BBF-CAEMs might be appropriate for
pavements in cold climate whereas TBF-CAEMs would be effective in road pavements exposed
to severe conditions both in hot and cold climates.
Keywords: Cold Asphalt Emulsion Mixtures; Blended fillers; Stiffness modulus; Repeated load
axial test; Durability; Microstructure; Delay hydration process
Nowadays, environmental issues about reducing energy consumption, reducing CO2 emissions
and managing wastes are being increasingly articulated and have been gaining attention
worldwide. One of the most significant trends towards more eco-friendly asphalt mixes is the
use of material such as recycled asphalt pavement, municipal solid waste incineration ash,
construction and demolition waste material, cement kiln dust and coal ash [1-8].
Due to the many significant environmental and economic benefits that can be derived from using
cold asphalt mixtures (CAMs), several research projects have been performed to study and
develop the properties of these mixtures. The development of CAMs has commonly been by
utilizing waste material/ by-products while achieving satisfactory hot mix asphalt (HMA)
properties [6, 7, 9, 10]. However, CAMs for sustainable and resilient pavements still has to meet
the requirements of carrying heavy traffic loads from a mechanical perspective. Additionally, the
properties of CAMs need to resist the impact of the environment from a durability perspective.
In the current research, these two features will be termed as engineering properties. The
enhancement of the engineering properties of CAMs mainly depends on the type, quantity and
quality of the raw materials used. This might be considered as one of the most important factors
to extend the use of CAMs for the use as a surface course.
Fillers can play a major role controlling the engineering properties of asphalt mixtures. It has
been demonstrated that filler can significantly influence permanent deformation resistance,
stiffness, fracture resistance, and moisture susceptibility of asphalt concrete [11, 12]. A recent
development aimed at achieving excellent engineering properties of CAMs is the use of
manufactured fillers. This kind of filler is produced as a blend of reactive, semi-reactive and
non-reactive natural fillers [6, 7, 13, 14]. In this study, binary blended fillers (BBFs) contain a
combination of fly ash (FA) or granulated blast furnace slag (GGBS) with ordinary Portland
cement (OPC), while the ternary blended fillers (TBFs) are a combination of BBFs with silica
fume (SF). These fillers are used for many reasons. FA, GGBS, SF are considered to be some of
the most used supplementary cementitious material alternatives. Furthermore, their availability
worldwide in substantial quantities can provide social, economic, and environment benefits.
An experimental study by Oruc, Celik and Akpinar  assessed the mechanical properties of
emulsified asphalt mixtures including 0-6% OPC, which was substituted for mineral filler. Their
findings showed a remarkable improvement with a high percentage of OPC treatment,
recommending these mixtures to be used as a structural layer. Al-Busaltan, Al Nageim, Atherton
and Sharples  confirmed the enhancement of close graded CAEM to a stage where its
mechanical properties were comparable to those of traditional asphalt concrete mixtures. The
improvement was due to the replacement of the conventional mineral filler with a domestic fly
ash. Al-Hdabi, Al Nageim, Ruddock and Seton  showed a significant improvement in
mechanical properties and water damage resistance of cold rolled asphalt by incorporating a
biomass fly ash with cement. Recently, the influence of chemical additives including OPC,
hydrated lime (HL), and a combination of HL and GGBS on recycled mixture performance was
investigated by Du . The results showed that hydration products can increase the stiffness
and cohesion of the asphalt mastic of the recycled mixture .
A comparison study between using coal ash and OPC in cold recycled asphalt mixtures was
carried out by Modarres and Ayar . The results revealed that the application of coal waste
powder improved the mechanical properties of cold recycled asphalt material, but it could not
achieve a positive impact on moisture damage resistance. Based on these comparisons, coal ash
was found to have comparable effects to OPC. While previous studies have highlighted the
importance of using OPC, HL and some specific kinds of fly ash in developing CAMs, there is
a need to develop more sustainable CAMs using artificial by-products such as FA, GGBS and
SF in combination with OPC. The purpose is to reduce the potential increase in production costs
and environmental issues particularly in the manufacturing process of both cement and lime.
However, the availability of alternative cement materials should be considered when choosing
the type of fillers in CAMs.
Pouliot, Marchand and Pigeon  showed that the presence of a small quantity of bitumen
emulsion in cement mortar had a delaying effect on the cement hydration. Furthermore, Du 
agreed with this study and proposed a mechanism for the hydration process delay. He suggested
that some of the bitumen droplets and cement particles come into contact due to intensive
chemical adsorption, and as a result, some of the cement particles are encapsulated by an asphalt
film, causing a delay or interruption in the hydration reaction. A study carried out by Wang, Shu,
Rutherford, Huang and Clarke  showed that the total hydration heat decreased with an
increase in bitumen to cement ratio in CAEM. Also, the study revealed that the addition of
bitumen emulsion significantly influenced cement hydration behaviour in CEAM. In contrast, a
recent experimental study carried out by Fang, Garcia, Winnefeld, Partl and Lura  revealed
that the behaviour of bitumen emulsion in the presence of cement and filler is still unclear and
may slightly retard or accelerate cement hydration, but has no significant effect on the degree of
cement hydration. These research studies have demonstrated developments in the properties of
CAEMs by using different types of filler. However, this raises an important question as to how
these fillers (cement/artificial by-products) interact with bitumen emulsion and affect the
hydration and microstructural characteristics of CAEMs.
2. Research significance
This study aims to develop special types of CAEM by using artificial by-products such as FA,
GGBS and SF in combination with OPC. Accordingly, it is hoped that wider utilization of
CAEMs in the construction of highway and pavement materials (with both environmental and
economic impacts) can be derived from the current research. Meanwhile, this work is designed
to contribute to a deeper understanding of the microstructure and internal composition of the
3. Material and testing program
3.1. Material characteristics
The aggregate used in this study was crushed limestone. The physical properties of the aggregate
were: apparent density 2.70 Mg/m3; absorption 0.4%; Los Angeles Coefficient 28. The gradation
of the aggregate was within the limits of 0/14 mm size close graded surface course, according to
BS EN 13108-1. This selection was made in order to ensure an appropriate interlock between the
aggregate particles in the mixtures as recommended by the European Stand